Sinter is a blast furnace input material obtained by temperature to 900-1200 oC without full melting and adhering to each other with superficial melting. It is considered as a multi-phase material with its heterogeneous microstructure. In general, the main mineral phases are hematite, magnetite, silicoferrite of calcium and aluminium (SFCA) and silicates. By determining the SFCA structure in the sinter material, the sintering process will be made more stable and important parameters affecting the quality in the sintering process will be examined. Sinter material consists of iron ore, iron and steel industry by-products and auxiliary materials. The scope of this project is the determination of the amount of SFCA formed by bonding SiO2, CaO, Fe2O3, Al2O3 and MgO compounds and monitoring this value as a parameter by sinter manufacturers. Sinter samples having different characteristic features were made ready for Xray diffraction (XRD) and optical microscopy inspections by polishing, etching and cold mounting in epoxy for mineralogical analyses. Before raw data obtained from the analysis were evaluated at Autoquan, they were converted into Autoquan format and then, read in XRD device and mineralogical composition of the sinter was revealed by XRD analyses. Detailed imaging of mineralogical compounds were made so as to complement scanning electron microscope (SEM) analyses and XRD analyses; elemental composition of the compounds and valence conditions of the elements were determined by energy dispersive spectroscopy (EDS) method. Phase structures such as hematite, magnetite, and calcium ferrite were qualitatively determined by mineralogical investigations on sinter samples. Furthermore, the variations of SFCA phases (SFCA, SFCA-I and SFCA-II) were studied through Rietveld method.
 R.P. Bhagat, U. Chattoray, and S.K. Sil, “Porosity of sinter and its relation with the sintering indices”, ISIJ International, vol. 46, no. 11, p. 1728-1730, 2006.
 T. Umadevi, R. Sah, and P. C. Mahapatra, “Influence of sinter basicity (CaO/SiO2) on low and high alumina iron ore sinter quality”, Mineral Processing and Extractive Metallurgy, 123(2), 75-85, 2014.
 R. Chaigneau, “Fluxed sinter formation and SFCA reduction under Simulated Conditions”, PhD Thesis, Delft University Press, p. 12-28, 1994.
 L.H. Hsieh and J.A. Whiteman, “Effect of oxygen potential on mineral formation in lime-fluxed iron ore sinter”, ISIJ International, vol. 29, no. 8, p. 625- 634, 1989.
 C. E. Loo, R. P. Williams, and L. T. Matthews, “Influence of material properties on high temperature zone reactions in sintering of iron ore”, Transactıons of The Institution of Mining And Metallurgy Sectıon C-Mineral Processing and Extractive Metallurgy, vol.101, p. 7-15, 1992.
 N. Chakraborti, K. Deb, and A. Jha, “A genetic algorithm based heat transfer analysis of a bloom re-heating furnace”, Steel Research, vol. 71, no. 10, p. 396-402, 2000.
 N. A. Webster, M. I. Pownceby, I. C. Madsen, and J. A. Kimpton, “Silico-ferrite of calcium and aluminum (SFCA) iron ore sinter bonding phases: new insights into their formation during heating and cooling”, Metallurgical and Materials Transactions B, 43(6), 1344-1357, 2012.
 N.J. Bristow and A.G. Waters, “Role of SFCA in promoting high-temperature reduction properties of iron ore sinters”. Mineral Processing & Extractive Metallurgy, Section C. vol. 100. p. 1-4, 1991.
 S. Nicol, J. Chen, M. I. Pownceby, and N. A. Webster, “A Review of the Chemistry, Structure and Formation Conditions of Silico-Ferrite of Calcium and Aluminum (SFCA) Phases”, ISIJ International, 58(12), 2157-2172, 2018.
 T. Takayama, R. Murao, and M. Kimura, “Quantitative Analysis of Mineral Phases in Iron-ore Sinter by the Rietveld Method of X-ray Diffraction Patterns”, ISIJ International, ISIJINT-2017, 2018.
 M. Kama, T. Miyazaki, K. Ito, Y. Hida, and M. Sasaki, “Morphological analysis of calcium ferrite and hematite in sintered ore”, Transactions ISIJ. vol. 24, 1984.
 W.G. Mumme, “The crystal structure of SFCA-II, Ca5.1Al9.3Fe3+ 14.30Fe2+ 0.55O48, a homologue of the aenigmatite structure type, and new structure type, and new crystal refinement of SFCA, Ca2Al5Fe7O20”, Implications for the nature of the ternary-phase solid-solution previously reported in the CaO-Al2O3-iron oxide system, Neues Jahrbuch Miner. Abh., vol. 178, no. 3, p.307-335, 2003.
 M. I. Pownceby, N. A. S. Webster, J. R. Manuel, and N. Ware, “The influence of ore composition on sinter phase mineralogy and strength”, Mineral Processing and Extractive Metallurgy, 125(3), 140-148, 2016.
 W.G. Mumme, J.M.F. Clout, and R.W. Gable, “The crystal structure of SFCA-I Ca3.18Fe3+ 14.66Al1.34Fe2+ 0.82O28, a homologue of the aenigmatite structure type, and new structure type, and new crystal refinements of β-CCF, Ca2.99Fe3+ 14.30Fe2+ 0.55O25 and Mg-free SFCA, Ca2.45Fe3+ 9.04Al1.74Fe2+ 0.16Si0.6O20”. Neues Jahrbuch Miner. Abh, vol. 173, no. 1, p. 93-117, 1988.
 M. I. Pownceby and J.M.F. Clout, “Importance of fine iron ore chemical composition and high temperature phase relations, applications to iron ore sintering and pelletizing”, Mineral Processing and Extractive Metallurgy, vol. 112, p. 44-51, 2003.
 W. Wang, X. H. Chen, R. S. Xu, J. Li, W. J. Shen, and S. P. Wang, “Research progress on multiscale structural characteristics and characterization methods of iron ore sinter”, Journal of Iron and Steel Research International, 1-13, 2020.
 R. Mežibrický, M. Fröhlichová, R. Findorák, and V. S. Goettgens, “Ore Assimilation and Secondary Phases by Sintering of Rich and High-Gangue Iron Ores”, Minerals, 9(2), 128, 2019.
 T. Harvey, “Influence of Mineralogy and Pore Structure on the Reducibility and Strength of Iron Ore Sinter”, Doctoral dissertation, University of Pretoria, Republic of South Africa, 2020.
 M. A. Nyembwe, “Study of sinter reactions when fine iron ore is replaced with coarse ore, using an infrared furnace and sinter pot tests”, Doctoral dissertation, The University of Newcastle, Australia, 2012.
 D. Fernández-González, I. Ruiz-Bustinza, J. Mochón, C. González-Gasca, and L. F. Verdeja, “Iron ore sintering: Process”. Mineral Processing and Extractive Metallurgy Review, 38(4), 215-227, 2017.
 A. Cores, L. F. Verdeja, S. Ferreira, I. Ruiz-Bustinza, and J. Mochon, Editor's Page: “Iron ore sintering. Part 1. Theory and practice of the sintering process”, Rev. Avances en Sistemas Informática, 10 (1), 152-171, 2013.
 S. Blake, R.G. Launsby, and D. L. Weese, “Experimental design meets the realities of the 1990s”, Quality Progress, p.99-101, 1994.
 P.R Dawson, J. Ostwald, and K.M. Hayes, “The influence of sintering temperature profile on the mineralogy and properties of iron ore sinters”, Proc. Aust. Inst. of Mining and Metallurgy, p. 163-169,1984.
 A. Cores, A. Babich, M. Muñiz, S. Ferreira, and J. Mochon, “The influence of different iron ores mixtures composition on the quality of sinter”, ISIJ International, vol. 50 , no. 8, p. 1089-1098, 2010.
 M.S. De Magalhaes and P.R.G. Brandao, “Microstructures of industrial sinters from Quadrilatero Ferrifero’s iron ores”, Minerals Engineering, Elsevier, p.1251, 2003.
 M. I. Pownceby and T.R.C. Patrick, “Stability of SFC (silico-ferrite of calcium): solid solution limits, thermal stability and selected phase relationships within the Fe2O3-CaOSiO2 (FCS) system”. European Journal of Mineralogy. vol. 12. p. 455-468, 2000.
 N. V. Y. Scarlett, M. I. Pownceby, I. C. Madsen, and A. N. Christensen, “Reaction sequences in the formation of silico-ferrites of calcium and aluminum in iron ore sinter”, Metallurgical and materials transactions B, vol. 35B, p. 929- 936, 2004.
 Y. Ishikawa, Y. Shimomura, M. Sasaki, and H. Toda, “Improvement of sinter quality based on the mineralogical properties of ores”, Ironmaking Proceedings. vol. 42. p. 17-29, 1983.
 L. X. Yang and E. Matthews, “Sintering reactions of magnetite concentrates under various atmospheres”, ISIJ International, vol. 37, no. 11, p. 1057-1065, 1997.
 S. Nicol, E. Jack, and P. C. Hayes, “Controlled Solidification of Liquids within the SFC Primary Phase Field of the Fe2O3-CaO-SiO2 System in Air”, Metallurgical and Materials Transactions B, 50(6), 3027-3038, 2019.
 N.V.Y. Scarlett, M. I. Pownceby, I. C Madsen, and A. N. Christensen, “In situ X-ray diffraction analysis of iron ore sinter”, Journal of Applied crystallography, vol. 37, no. 3, p. 362-368, 2004.
 P. Łechtańska and G. Wielgosiński, “The use of ammonium sulfate as an inhibitor of dioxin synthesis in iron ore sintering process”, Ecological Chemistry and Engineering, 2014.
 R. A. Young, “The Rietveld method, International Union Crystallography”, Oxford University Press, Oxford, 298p, 1993.